IOSR Journal of Applied Physics (IOSR-JAP)e-ISSN: 2278-4861. Volume 3, Issue 1 (Jan. - Feb. 2013), pp 01-06www.iosrjournals.orgwww.iosrjournals.org 1 | PageStudy of Dielectric Properties of Nano-crystalline Mn-Zn FerriteSunita Bhagwat*, Pratibha RaoDepartment of Physics, Abasaheb Garware College, Karve Road, Pune – 411 004, IndiaAbstract: The ac conductivity σ and dielectric properties (dielectric constant ’, dielectric loss ’’ and losstangent tan δ) were measured as a function of frequency between 100 Hz and 20 MHz for the mixed ferritesZnxMn1-xFe2O4 (where x = 0.2 to 0.8), synthesized by solid-state route. The ac conductivity σ below 1 MHzseems to be nearly frequency independent for all compositions; and above these frequency ranges, σ sharplyincreases until it reaches a maximum value. The relaxation time (τ) was found to be in the range 0.3x10-5–1.5x10-5sec from the hopping frequency. The dielectric constant for these ferrites is approximately inverselyproportional to the square root of the resistivity. The electrical conduction mechanism was explained in terms ofthe electron hopping model. The formation of spinel structure and crystalline size was confirmed using X-raydiffraction (XRD) technique. Morphology of the samples was studied using Scanning Electron Microscopy(SEM).Keywords: Solid-state route; spinel ferrite; dielectric properties; ac conductivityI. INTRODUCTIONPolycrystalline spinel ferrites are known for their sensing applications [1-2] apart from their everincreasing demand in the technological applications in microwave and radio wave devices. These ferrites arewidely used for manufacturing transformers and inductors in power supplies . They are mainly classified intwo categories: the high permeability ferrites which are used for filtering applications and the low core lossferrites used for power transformers and inductors in switching mode power supplies. Mn-Zn ferrites are knownfor magnetic sensors . However, they have not been explored much for microwave applications. The ferriteresonator antennas (FRAs) have the ability to change their characteristics as a function of the applied magneticfield. The low dielectric behaviour makes ferrite materials useful in high frequency applications. Some of theproperties of dielectric resonator antennas (DRAs) can be actively controlled using low-loss ferrite materials .In the present work polycrystalline samples of ZnxMn1-xFe2O4 (x ranges from 0.2 to 0.8) were preparedby solid-state route. The structural characterization was studied using XRD. The morphological studies werecarried out using SEM.II. EXPERIMENTAL2.1 Synthesis TechniquePolycrystalline samples of ZnxMn1-xFe2O4 (x ranges from 0.2 to 0.8) were prepared by solid-state routeusing high purity ZnO, Fe2O3 and MnCO3 respectively in stoichiometric proportions. The ZnO/Fe2O3 andMnCO3/Fe2O3 powders were grounded separately for 30 min using an agate mortar. Each mixture wastransferred to a ball mill for 6h using 50 ml vials and 12 mm diameter balls made of stainless steel and a ball-to-powder mass ratio of 20. A rotation speed of 240 rpm was used. The milling was done in air atmosphere withoutany additives. The powder is calcinated at 1000oC for 1h with a heating rate of 2oC/min followed by cooling atroom temperature in air. The pre-sintered samples were crushed again and mixed for another 30 min. withacetone, to be reduced into small crystallites of uniform size. The mixture was air dried and a proper proportionof each powder was again ball milled by adding few drops of 2-propanol. The milling was done with theintention of producing a homogenous mixture of both solid components, without provoking significantstructural damage. Finally, the milled reactive powders were dried at 80oC in a furnace for 30 min. The powderwas compressed uniaxially under a pressure of 1x107N/m2into pellet form of diameter 10 mm and thicknessabout 2 mm. The pellets were sintered at 1000oC for 3 h in air atmosphere and cooled to room temperature tomake them rigid and impart ceramic properties.2.2 Characterization TechniquesThe structural characterization of the ferrite samples was carried out using Philips diffractometer, withCuK radiation. The average crystallite size, t, was determined using the Scherrer formula :t = 0.9 / B1/2 cos b (1)where B1/2 is the angular line width at half maximum intensity and b is the Bragg angle for the actual peak.
Study of Dielectric Properties of Nano-crystalline Mn-Zn Ferritewww.iosrjournals.org 2 | PageDielectric measurements were carried out at room temperature using 4192A impedance analyzer over awide range of frequency from 100 Hz up to 20 MHz. The dielectric constant ’ were calculated using theformula:’ = Cd / oA (2)where o the permittivity of the free space, C is the capacitance, d the thickness and A the cross-sectional area ofthe pellet.The dielectric loss factor ’’ has been calculated from the relation:’’ = ’ tan (3)where tan is the loss tangent.The ac conductivity σ of the sample was determined from dielectric parameters using the relationac = ’’ (4)where is the angular frequency.III. RESULTS AND DISCUSSION3.1 X-ray diffraction StudiesFig.1 shows the typical X-ray diffraction pattern for ZnxMn1-xFe2O4 compact disk sintered at 1000oC inair for 3 h. The XRD pattern exhibits all the peaks indicative of single phase spinel crystal structure. The non-occurrence of the other phases suggests there is no solubility limit to Zn2+ions in the manganese ferrite spinellattice. It is known that the degree of replacement of the host cations by the other ions in the host lattice dependson the cation radius of the substituent . The crystallite size of all the samples was calculated using theScherrer formula and it was found to be between 40 and 50 nm.20 30 40 50 60 70 80(440)(511)(422)(400)(220)Intensity(Arbitaryunits)2 (deg)(311)Figure 1: Typical XRD pattern of ZnxMn1-xFe2O43.2 Dielectric Constant BehaviourThe dielectric behaviour of ferrite nanoparticles are influenced mainly by the synthesis technique, grainsize, cation distribution etc . The behavior of both ’, ’’ and σ at RT versus frequency are shown in Fig.2 (a-e). The general trend for all composition is that ’ and ’’ decrease with increasing frequency. The decrease indielectric constant with increasing frequency is attributed to the fact that electron exchange between Fe2+andFe3+ions cannot follow the change of the external applied field beyond certain frequency . At lowerfrequencies the grain boundaries are more effective than grain electrical conduction. This behavior of adielectric constant, with Zn ions substitution can be explained qualitatively on the basis of the mechanism of thepolarization process in ferrite which is similar to that in the conduction process. The whole polarization inferrites is mainly contributed by the space charge polarization, which is governed by the number of space chargecarriers. The conductivity in the material and the hopping exchange of charges between two localized statesgoverned by density of the localized state and resultant displacement of charges w.r.t. the external field. As thefrequency increases ionic and orientation sources of polarizability decrease and finally disappear due to inertiaof the molecules and ions. The high value of the dielectric constant in the present ferrite for x = 0.2 may beattributed to space charge polarization ; or it could be due to an increase in crystallite size andmorphologically clean microstructure as seen in Fig. 3(a).
Study of Dielectric Properties of Nano-crystalline Mn-Zn Ferritewww.iosrjournals.org 3 | PageAn examination of Table I reveals that the values of dielectric constant ’, dielectric loss ’’ and losstangent tan δ are maximum for x = 0.2. It also can be seen that among these mixed Mn–Zn ferrites, the one withthe compositions Zn0.8Mn0.2Fe2O4 exhibits the lowest dielectric constant, the lowest dielectric loss, the lowestloss tangent and the lowest electrical conductivity. This might be due the presence of macro-agglomerationscontaining very fine particles which can be clearly seen in Fig. 3(b).From Table I it can be seen that the composition Zn0.2Mn0.8Fe3O4 has the maximum dielectric constant(47.9). This high value can be explained as it has maximum number of ferrous ions whose exchange betweenFe2+and Fe3+gives rise to maximum dielectric polarization, that could be due to the availability of ferrous ionson octahedral B - site. It is also pertinent to mention that the variation of electrical conductivity runs parallel tothe variation in dielectric constant as shown in Fig.2. Thus, it is the number of ferrous ions on octahedral sitesthat play a dominant role in the processes of conduction as well as dielectric polarization. The electricalconduction mechanism can be explained by the electron hopping model of Heikes and Johnston . Oneobtains local displacements of electrons in the direction of the applied electric field; these displacementsdetermine the polarization of the ferrite.Table I. Dielectric data of ZnxMn1-xFe2O4 at 100 kHz3.3 Dielectric Loss FactorAll dielectric materials have two types of losses. One is a conduction loss, representing the flow ofactual charges through the dielectric material. The other dielectric loss is due to the movement or rotation of theatoms in an alternating field. The dielectric loss factor ’’ with variation in frequency is as shown in Fig.2. It isconsidered to be the most important part of the total core loss in ferrites. The dielectric loss pattern is seen to besimilar to that of dielectric constant. This dielectric loss factor is attributed to domain wall resonance. At higherfrequencies, losses are found to be low, if domain wall motion is inhibited and magnetization is forced to changeby rotation. The dielectric loss obtained for the present nano-ferrites synthesized by solid-state method possesslower value for x = 0.8 which makes this ferrite to be useful in the higher frequency applications like DRAs.3.4 Dielectric Loss TangentFig. 2(f) shows the variation of the loss tangent tan δ with frequency for the investigated composition.It is known that loss tangent tan δ is defined as ’’/’. The occurrence of peaks in the variation of loss tangentwith frequency can observed when the hopping frequency of localized charge carriers is approximately equal tothat of the externally applied electric field; i.e., resonance phenomena. From the Fig.2 (f) it can be seen thatbetween x = 0 and 0.8 tan shows a maximum at frequency between 10 and 50 kHz. Iwauchi  reported astrong correlation between the conduction mechanism and the dielectric behaviour of the ferrites. Theconduction mechanism in n-type ferrites is considered as due to hopping of electrons between Fe2+and Fe3+resulting in local displacements which determines the polarization behaviour of the ferrites . The conditionfor observing a maximum in tan δ of a dielectric material is given by :τ ~1 (4)where is the relaxation time.And = 2πfmax, where fmax is proportional to the hopping probability p. The relaxation time is relatedto the hopping probability per unit time, p, by an equation p or fmax α p. It was found to be in the range0.3x10-5– 1.5x10-5sec. A decrease of fmax with increasing zinc content indicates that the hopping probability perunit time decreases continuously except for x = 0.65.3.5 AC ConductivityThe ac conductivity σ and dielectric properties (’ and ’’) as a function of frequency at RT for theabove mentioned composition are shown in Fig.2 (a–e). It can be seen that below 1 MHz, σ seems to be nearlyfrequency independent for all compositions. Above these frequency ranges, σ sharply increases until it reaches amaximum value. The dispersion in σ with frequency has been explained by Koop’s theorem  whichsuggested that the ferrite compact acts as multilayer capacitor. In this model, the ferrite grains and grainx [/-cm] tan [-cm] sqrt () *sqrt()0.2 4.79E+01 8.82E+01 5.04E-06 1.84E+00 1.98E+05 445.4354 2.13E+040.35 1.27E+01 1.06E+01 6.06E-07 7.77E-01 1.65E+06 1284.174 1.63E+040.5 2.38E+01 1.86E+01 1.06E-06 7.82E-01 9.41E+05 969.8687 2.31E+040.65 1.07E+01 4.14E+00 2.37E-07 3.86E-01 4.23E+06 2055.508 2.20E+040.8 5.45E+00 3.59E-01 2.05E-08 6.58E-02 4.88E+07 6986.689 3.81E+04a
Study of Dielectric Properties of Nano-crystalline Mn-Zn Ferritewww.iosrjournals.org 4 | Pageboundaries have different properties. The effect of the multilayer condenser rise with frequency as a result theconductivity increases.2 3 4 5 6 7020406080100log fConductivityx10-6(/Ohm-cm)050010001500200025003000andx = 0.2 a2 3 4 5 6 7020406080log fConductivityx10-6(/Ohm-cm)x = 0.35 b020040060080010001200and2 3 4 5 6 70204060Conductivityx10-6(/Ohm-cm)log f02004006008001000andx = 0.5c2 3 4 5 6 70204060log fConductivityx10-6(/Ohm-cm)010203040andx = 0.65 d2 3 4 5 6 70204060log fx = 0.802468101214Conductivityx10-6(/Ohm-cm)ande2 3 4 5 6 70.00.40.81.21.62.0tanlog fx = 0.2x = 0.5x = 0.65x = 0.8x = 0.35fFigure 2: (a-e) plot of ’,’’ and σ vs. frequency and (f) tan vs. frequency at room temperatureFigure 3: SEM micrographs of ZnxMn1-xFe2O4 samples for (a) x = 0.2 and (b) x = 0.8ba
Study of Dielectric Properties of Nano-crystalline Mn-Zn Ferritewww.iosrjournals.org 5 | Page3.6 Relation Between the Dielectric Constant and the ResistivityThe values of resistivity and are shown in Table 1. It can be seen from the table that the ’is roughly inversely proportional to the square root of resistivity and the product remains nearly constantas shown in the Table 1. A similar relationship between ’ and was found by Ravinder  for differentferrites. The dielectric losses in ferrites are generally reflected in the resistivity measurements, materials withlow resistivity exhibiting high dielectric losses and vice versa . Fig. 4 shows that the plot of dielectricconstant ’ vs. zinc content x is an inverse image of that of log of resistivity vs. zinc content. This is aconfirmation of the correlation between dielectric constant and resistivity .0.2 0.3 0.4 0.5 0.6 0.7 0.80204060Zn content (x)Dielectricconstantg5.05.56.06.57.07.58.0logFigure 4: Plot of dielectric constant and resistivity vs Zn concentrationIV. CONCLUSIONThe dielectric properties of Mn-Zn ferrites were investigated in this study and the results aresummarized as follows:1. The general trend for all composition is that ’ and ’’ decrease with increasing frequency.2. The value of the dielectric constant for the sample when x = 0.2 is found to be high due to space chargepolarization mechanism or could be due to morphologically clean grain structure.3. The value of the dielectric constant for the sample when x = 0.8 is found to be low which makes this ferriteto be useful in the higher frequency applications like DRAs.4. The frequency dependence of dielectric loss tangent (tanδ) shows the existence of broad peaks at lowfrequency range.5. The ’ is roughly inversely proportional to the square root of resistivity and the product remainsnearly constant.ACKNOWLEDGEMENTAuthor (SMB) is thankful to University Grants Commission (UGC), New Delhi for providing financialassistance. Authors are grateful to Dr. Jyoti Jog and Mr. Chetan Chanmal, National Chemical Laboratory, Punefor providing the dielectric data of the samples.REFERENCES Y. Chen, J. E. Snyder, C. R. Schwichtenberg, K. W. Dennis, R. W. McCallum, D. C. Jiles, Metal bonded Co-ferrite for torque sensorapplications, IEEE Transactions on Magnetics, 35, 1999, 3652-3654. N. Iftimie, E. Rezlusu, P. D. Popa, N. Reslescu, Gas sensitivity of nano-crystalline nickel ferrite, Journal of Optoelectronics andAadvance Materials, 8, 2006, 1016-1018. M. Sugimoto, The past, present and future of ferrites, Journal of American Ceramics Society, 82, 1999, 269-280. R. Lebourgeois, C. Coillot, Mn-Zn ferrites for magnetic sensor in space application, Journal of Applied Physics, 103, 2008, 07E510-513. P. B. A. Fechine, R. S. T. Moretzsohn, R. C. S. Costa, J. Derov, J. W. Stewart, A. J. Drehman, C. Junqueira, A. S. B. Sombra,Dielectric ferrite resonator antennas, Microwave and Optical Technology Letters, 50, 2008, 2852–2857. H. P. Klug and L. E. Alexander, X-ray Diffraction Procedures for Polycrystalline and Amorphous Materials ( John Wiley, New York,1974) 491. D. J. Kim, Lattice parameters, ionic conductivities and solubility limits in fluorite-structure MO2 oxide [M = Hf4+, Zr4+, Ce4+, Th4+,U4+] solid solutions, Journal of American Ceramics Society, 72, 1989, 1415-16. H.M. Abdelmoneim, Dielectric properties of TixLi1-xLa0.1Fe1.9O4 ferrite thin films, Indian Jornal of Pure and Appied. Physics, 48,2010, 562-570. G. Ranga Mohan, D. Ravinder, A.V. Ramana Reddy and B.S. Boyanov, Dielectric properties of polycrystalline mixed nickel–zincferrites, Materials Letters, 40, 1999, 39-45.
Study of Dielectric Properties of Nano-crystalline Mn-Zn Ferritewww.iosrjournals.org 6 | Page D.El. Kony, Dielectric Relaxation in Al-substituted Ni-Cd spinel ferrites, Egyptcian Journal of Solids, 27, 2004, 285-297. R.R. Heikes and D. Johnston, Jornal of Chemical Physics, 26, 1957, 582. K. Iwauchi, Journal of Applied Physics, 10, 1960, 1520. L.I. Rabinkin and Z.I. Novika (Ferrites Minsk, 1960) 146. M. B. Reddy and P.V. Reddy, Journal of Physics D: Applied Physics, 24, 1991, 975. C.G. Koops, On the dispersion of resistivity and dielectric constant of some semiconductors at audio frequencies, Physical Review, 83,1951, 121-124. D. Ravinder, Dielectric behaviour of lithium-cadmium ferrites, Physica Status Solidi A, 129, 1992, 549-554. A.S. Hudson, Marconi Review, 37, 1968, 43.